#------------------------------------------------------------------------------
#$Date: 2021-06-11 11:03:55 +0300 (Fri, 11 Jun 2021) $
#$Revision: 266400 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/33/1563349.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1563349
loop_
_publ_author_name
'Hussain, Firasat'
'Sandriesser, Stefan'
'Speldrich, Manfred'
'Patzke, Greta R.'
_publ_section_title
;
 A new series of lanthanoid containing Keggin-type germanotungstates with
 acetate chelators: [{Ln(CH3COO)GeW11O39(H2O)}2]12− {Ln=EuIII,
 GdIII, TbIII, DyIII, HoIII, ErIII, TmIII, and YbIII}
;
_journal_issue                   1
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              214
_journal_page_last               219
_journal_paper_doi               10.1016/j.jssc.2010.11.005
_journal_volume                  184
_journal_year                    2011
_chemical_formula_sum            'C4 H6 Ge2 K8 Na4 O110 Tb2 W22'
_chemical_formula_weight         6726.57
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 110.886(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   20.1171(5)
_cell_length_b                   12.6768(2)
_cell_length_c                   21.1300(5)
_cell_measurement_reflns_used    8267
_cell_measurement_temperature    183(2)
_cell_measurement_theta_max      29.4139
_cell_measurement_theta_min      2.5268
_cell_volume                     5034.5(2)
_computing_cell_refinement       'CrysAlis RED (Oxford, 2007)'
_computing_data_collection       'CrysAlis RED (Oxford, 2007)'
_computing_data_reduction        'CrysAlis RED (Oxford, 2007)'
_computing_molecular_graphics    'ORTEP-3 (Farrugia, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      183(2)
_diffrn_detector_area_resol_mean 10.4498
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Xcalibur, Ruby'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0953
_diffrn_reflns_av_sigmaI/netI    0.1092
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            43134
_diffrn_reflns_theta_full        25.68
_diffrn_reflns_theta_max         25.68
_diffrn_reflns_theta_min         2.53
_exptl_absorpt_coefficient_mu    27.460
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.27940
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.41 (release 06-05-2009 CrysAlis171 .NET)
(compiled May  6 2009,17:20:42)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    4.437
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       diamondshape
_exptl_crystal_F_000             5856
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.03
_refine_diff_density_max         8.890
_refine_diff_density_min         -3.029
_refine_diff_density_rms         0.451
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.942
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     401
_refine_ls_number_reflns         9548
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.942
_refine_ls_R_factor_all          0.0852
_refine_ls_R_factor_gt           0.0461
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0317P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0882
_refine_ls_wR_factor_ref         0.0948
_reflns_number_gt                6099
_reflns_number_total             9548
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2011-184-214.cif
_cod_data_source_block           fh124
_cod_original_cell_volume        5034.51(19)
_cod_database_code               1563349
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W8 W 0.28360(4) 0.92022(6) 0.38253(3) 0.01110(18) Uani 1 1 d . . .
W7 W 0.21085(4) 1.33624(6) 0.14709(4) 0.01290(19) Uani 1 1 d . . .
W6 W 0.12947(4) 1.32894(6) 0.25989(3) 0.01253(18) Uani 1 1 d . . .
W5 W 0.37421(4) 0.92655(6) 0.26008(3) 0.01097(18) Uani 1 1 d . . .
W4 W 0.16247(4) 1.10601(6) 0.37966(3) 0.01183(18) Uani 1 1 d . . .
W1 W 0.30821(4) 1.30438(6) 0.40241(3) 0.01184(18) Uani 1 1 d . . .
Ge1 Ge 0.25494(11) 1.12919(14) 0.26642(9) 0.0093(4) Uani 1 1 d . . .
W10 W 0.12246(4) 0.92791(6) 0.25368(3) 0.01140(18) Uani 1 1 d . . .
W9 W 0.21440(4) 0.93956(6) 0.12904(3) 0.01208(18) Uani 1 1 d . . .
W2 W 0.08553(4) 1.15160(6) 0.13045(3) 0.01248(18) Uani 1 1 d . . .
W3 W 0.33787(4) 1.12595(6) 0.14590(3) 0.01172(18) Uani 1 1 d . . .
W11 W 0.38897(4) 1.31960(6) 0.29068(3) 0.01146(18) Uani 1 1 d . . .
Tb1 Tb 0.45289(5) 1.11199(7) 0.42565(4) 0.0114(2) Uani 1 1 d . . .
O11 O 0.4586(7) 0.7764(9) 0.4963(6) 0.018(3) Uiso 1 1 d . . .
O10 O 0.4326(7) 0.8198(9) 0.2712(5) 0.014(3) Uiso 1 1 d . . .
O9 O 0.1732(8) 0.8584(10) 0.0616(6) 0.028(3) Uiso 1 1 d . . .
O8 O 0.3959(7) 1.0088(9) 0.1907(5) 0.013(3) Uiso 1 1 d . . .
O7 O 0.3876(7) 1.2415(9) 0.4556(5) 0.011(3) Uiso 1 1 d . . .
O6 O 0.1227(7) 1.2621(9) 0.0917(5) 0.017(3) Uiso 1 1 d . . .
O4 O 0.0826(6) 1.0465(8) 0.1959(5) 0.007(3) Uiso 1 1 d . . .
O3 O 0.1889(6) 0.8550(9) 0.3222(5) 0.012(3) Uiso 1 1 d . . .
O2 O 0.1724(7) 0.9003(9) 0.1942(5) 0.015(3) Uiso 1 1 d . . .
O1 O 0.1473(7) 1.0539(8) 0.1084(5) 0.011(3) Uiso 1 1 d . . .
K1 K 0.5278(2) 1.1185(3) 0.26872(19) 0.0196(10) Uani 1 1 d . . .
K2 K 0.1722(3) 1.1591(4) -0.0104(2) 0.0361(13) Uani 1 1 d . . .
K3 K 0.3099(3) 0.7377(4) 0.0686(2) 0.0355(13) Uani 1 1 d . . .
K4 K -0.0281(2) 1.1323(3) 0.2387(2) 0.0216(11) Uani 1 1 d . . .
Na1 Na 0.0932(5) 0.7439(6) -0.0202(4) 0.036(2) Uani 1 1 d . . .
O87 O 0.4503(7) 1.0350(9) 0.0170(5) 0.017(3) Uiso 1 1 d . . .
Na2 Na -0.0481(6) 0.5522(8) -0.0110(5) 0.057(3) Uani 1 1 d . . .
O46 O 0.5327(6) 0.9579(8) 0.4614(5) 0.007(3) Uiso 1 1 d . . .
O45 O 0.3528(7) 1.0138(9) 0.4134(5) 0.015(3) Uiso 1 1 d . . .
O44 O 0.0058(7) 1.1269(9) 0.0672(6) 0.020(3) Uiso 1 1 d . . .
O43 O 0.1179(6) 1.2096(8) 0.3139(5) 0.009(3) Uiso 1 1 d . . .
O42 O 0.0568(7) 1.2534(9) 0.1823(6) 0.019(3) Uiso 1 1 d . . .
O41 O 0.2093(7) 1.4338(9) 0.0923(5) 0.015(3) Uiso 1 1 d . . .
O39 O 0.4334(7) 1.4206(9) 0.2704(5) 0.018(3) Uiso 1 1 d . . .
O38 O 0.2913(7) 1.3615(9) 0.2190(5) 0.015(3) Uiso 1 1 d . . .
O37 O 0.4239(7) 1.0159(9) 0.3235(5) 0.012(3) Uiso 1 1 d . . .
O36 O 0.3840(6) 1.2155(8) 0.2187(5) 0.010(3) Uiso 1 1 d . . .
O35 O 0.2230(7) 0.9880(9) 0.4241(5) 0.012(3) Uiso 1 1 d . . .
O34 O 0.3217(6) 1.2032(8) 0.3222(5) 0.006(3) Uiso 1 1 d . . .
O33 O 0.3581(6) 1.3900(9) 0.3563(5) 0.012(3) Uiso 1 1 d . . .
O32 O 0.5674(7) 1.0801(9) 0.4069(6) 0.017(3) Uiso 1 1 d . . .
O31 O 0.2866(6) 1.0502(9) 0.2143(5) 0.011(3) Uiso 1 1 d . . .
O30 O 0.0547(7) 0.8383(9) 0.2282(5) 0.017(3) Uiso 1 1 d . . .
O29 O 0.2415(7) 1.1982(9) 0.4103(5) 0.013(3) Uiso 1 1 d . . .
O28 O 0.4583(6) 1.2484(9) 0.3506(5) 0.010(3) Uiso 1 1 d . . .
O27 O 0.2957(7) 1.3989(9) 0.4560(6) 0.018(3) Uiso 1 1 d . . .
O26 O 0.2694(7) 1.0254(9) 0.0897(5) 0.014(3) Uiso 1 1 d . . .
O25 O 0.1882(6) 1.2101(8) 0.2137(5) 0.010(3) Uiso 1 1 d . . .
O24 O 0.3128(7) 0.8156(9) 0.4395(5) 0.017(3) Uiso 1 1 d . . .
O23 O 0.3153(7) 0.8823(9) 0.3090(5) 0.014(3) Uiso 1 1 d . . .
O22 O 0.3827(7) 1.1567(9) 0.0930(5) 0.017(3) Uiso 1 1 d . . .
O21 O 0.2149(7) 1.0428(9) 0.3073(5) 0.013(3) Uiso 1 1 d . . .
O20 O 0.1210(7) 1.1329(9) 0.4360(5) 0.017(3) Uiso 1 1 d . . .
O19 O 0.2961(7) 0.8666(9) 0.1764(5) 0.017(3) Uiso 1 1 d . . .
O18 O 0.1518(7) 1.4051(9) 0.1915(6) 0.019(3) Uiso 1 1 d . . .
O17 O 0.2163(6) 1.3502(9) 0.3218(5) 0.010(3) Uiso 1 1 d . . .
O16 O 0.0772(7) 1.4253(10) 0.2772(6) 0.020(3) Uiso 1 1 d . . .
O15 O 0.2618(7) 1.2268(9) 0.1193(5) 0.014(3) Uiso 1 1 d . . .
O14 O 0.0981(7) 1.0040(9) 0.3224(5) 0.017(3) Uiso 1 1 d . . .
C1 C 0.5745(10) 0.9922(14) 0.4319(8) 0.013(4) Uiso 1 1 d . . .
C2 C 0.6341(11) 0.9183(15) 0.4300(9) 0.024(5) Uiso 1 1 d . . .
H2A H 0.6300 0.9069 0.3839 0.035 Uiso 1 1 calc R . .
H2B H 0.6302 0.8520 0.4504 0.035 Uiso 1 1 calc R . .
H2C H 0.6794 0.9496 0.4546 0.035 Uiso 1 1 calc R . .
O86 O 0.1857(7) 0.6227(9) 0.0196(5) 0.013(3) Uiso 1 1 d . . .
O85 O 0.2697(7) 0.8883(10) -0.0323(6) 0.022(3) Uiso 1 1 d . . .
O84 O 0.4201(8) 0.8787(11) 0.0951(7) 0.037(4) Uiso 1 1 d . . .
O83 O 0.6756(8) 1.1056(11) 0.3185(7) 0.035(4) Uiso 1 1 d . . .
O82 O 0.0445(9) 1.0983(12) -0.0841(8) 0.051(5) Uiso 1 1 d . . .
O94 O 0.1317(9) 0.7994(11) -0.1112(7) 0.041(4) Uiso 1 1 d . . .
O93 O 0.0283(8) 0.5949(10) -0.0935(6) 0.027(3) Uiso 1 1 d . . .
O89 O -0.1069(8) 1.1145(11) 0.3213(7) 0.035(4) Uiso 1 1 d . . .
O88 O 0.0300(11) 0.7081(15) 0.0552(9) 0.074(6) Uiso 1 1 d . . .
O47 O 0.7579(9) 1.1827(11) 0.2513(7) 0.043(4) Uiso 1 1 d . . .
O49 O 0.4695(9) 0.6911(12) 0.3825(7) 0.043(4) Uiso 1 1 d . . .
O50 O 0.3359(9) 1.6006(12) 0.3695(7) 0.046(4) Uiso 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Tb Tb -0.1723 4.1537 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O24 W8 O45 103.2(5) . .
O24 W8 O23 103.8(5) . .
O45 W8 O23 91.2(5) . .
O24 W8 O35 97.8(5) . .
O45 W8 O35 94.3(5) . .
O23 W8 O35 155.9(5) . .
O24 W8 O3 97.6(5) . .
O45 W8 O3 159.2(5) . .
O23 W8 O3 84.3(5) . .
O35 W8 O3 82.3(5) . .
O24 W8 O21 164.1(5) . .
O45 W8 O21 90.1(5) . .
O23 W8 O21 84.4(4) . .
O35 W8 O21 72.1(4) . .
O3 W8 O21 69.3(4) . .
O41 W7 O38 103.8(5) . .
O41 W7 O15 101.5(5) . .
O38 W7 O15 88.3(5) . .
O41 W7 O18 97.8(5) . .
O38 W7 O18 91.9(5) . .
O15 W7 O18 160.1(5) . .
O41 W7 O6 98.6(5) . .
O38 W7 O6 157.6(5) . .
O15 W7 O6 86.5(5) . .
O18 W7 O6 85.8(5) . .
O41 W7 O25 168.2(5) . .
O38 W7 O25 85.5(5) . .
O15 W7 O25 85.9(4) . .
O18 W7 O25 74.2(4) . .
O6 W7 O25 72.4(4) . .
O41 W7 K2 83.5(4) . .
O38 W7 K2 132.2(4) . .
O15 W7 K2 44.5(3) . .
O18 W7 K2 134.5(4) . .
O6 W7 K2 49.5(4) . .
O25 W7 K2 95.8(3) . .
O16 W6 O17 104.2(5) . .
O16 W6 O18 97.3(5) . .
O17 W6 O18 92.6(5) . .
O16 W6 O43 102.4(5) . .
O17 W6 O43 88.7(5) . .
O18 W6 O43 159.3(5) . .
O16 W6 O42 100.9(6) . .
O17 W6 O42 154.8(5) . .
O18 W6 O42 85.6(5) . .
O43 W6 O42 84.5(5) . .
O16 W6 O25 168.3(4) . .
O17 W6 O25 84.0(5) . .
O18 W6 O25 73.8(4) . .
O43 W6 O25 85.9(4) . .
O42 W6 O25 71.4(5) . .
O16 W6 K4 86.9(4) . .
O17 W6 K4 135.7(4) . .
O18 W6 K4 129.0(4) . .
O43 W6 K4 47.0(3) . .
O42 W6 K4 44.1(3) . .
O25 W6 K4 92.9(3) . .
O10 W5 O37 102.9(5) . .
O10 W5 O23 102.4(5) . .
O37 W5 O23 94.0(5) . .
O10 W5 O8 101.1(5) . .
O37 W5 O8 90.5(5) . .
O23 W5 O8 154.3(5) . .
O10 W5 O19 95.8(5) . .
O37 W5 O19 161.0(5) . .
O23 W5 O19 85.7(5) . .
O8 W5 O19 81.9(5) . .
O10 W5 O31 163.7(4) . .
O37 W5 O31 91.3(5) . .
O23 W5 O31 84.2(5) . .
O8 W5 O31 70.5(5) . .
O19 W5 O31 69.7(4) . .
O10 W5 K1 89.6(4) . .
O37 W5 K1 48.5(4) . .
O23 W5 K1 142.5(3) . .
O8 W5 K1 47.2(3) . .
O19 W5 K1 128.7(3) . .
O31 W5 K1 94.0(3) . .
O20 W4 O43 98.7(5) . .
O20 W4 O29 101.3(5) . .
O43 W4 O29 86.7(5) . .
O20 W4 O14 100.7(6) . .
O43 W4 O14 88.2(5) . .
O29 W4 O14 157.8(5) . .
O20 W4 O35 101.1(5) . .
O43 W4 O35 160.1(5) . .
O29 W4 O35 90.2(5) . .
O14 W4 O35 87.3(5) . .
O20 W4 O21 171.0(5) . .
O43 W4 O21 87.9(4) . .
O29 W4 O21 85.1(4) . .
O14 W4 O21 73.2(5) . .
O35 W4 O21 72.3(4) . .
O20 W4 K2 48.7(4) . 4_586
O43 W4 K2 79.0(3) . 4_586
O29 W4 K2 56.2(4) . 4_586
O14 W4 K2 143.3(4) . 4_586
O35 W4 K2 115.3(3) . 4_586
O21 W4 K2 139.4(3) . 4_586
O20 W4 K4 85.7(4) . .
O43 W4 K4 46.2(4) . .
O29 W4 K4 132.8(3) . .
O14 W4 K4 47.6(4) . .
O35 W4 K4 134.6(3) . .
O21 W4 K4 94.6(3) . .
K2 W4 K4 102.91(11) 4_586 .
O27 W1 O7 101.7(5) . .
O27 W1 O29 99.0(5) . .
O7 W1 O29 97.3(5) . .
O27 W1 O33 99.3(5) . .
O7 W1 O33 93.4(5) . .
O29 W1 O33 156.4(4) . .
O27 W1 O17 92.8(5) . .
O7 W1 O17 165.5(5) . .
O29 W1 O17 80.0(5) . .
O33 W1 O17 84.4(5) . .
O27 W1 O34 171.2(5) . .
O7 W1 O34 84.1(4) . .
O29 W1 O34 86.7(4) . .
O33 W1 O34 73.5(4) . .
O17 W1 O34 81.5(4) . .
O27 W1 K2 46.0(4) . 4_586
O7 W1 K2 112.6(4) . 4_586
O29 W1 K2 53.9(3) . 4_586
O33 W1 K2 138.8(3) . 4_586
O17 W1 K2 77.5(3) . 4_586
O34 W1 K2 137.7(3) . 4_586
O34 Ge1 O25 110.7(5) . .
O34 Ge1 O21 112.8(5) . .
O25 Ge1 O21 107.3(6) . .
O34 Ge1 O31 111.7(5) . .
O25 Ge1 O31 107.6(5) . .
O21 Ge1 O31 106.5(5) . .
O30 W10 O3 100.9(5) . .
O30 W10 O2 102.7(5) . .
O3 W10 O2 91.2(5) . .
O30 W10 O4 102.4(5) . .
O3 W10 O4 156.6(5) . .
O2 W10 O4 85.6(5) . .
O30 W10 O14 100.4(5) . .
O3 W10 O14 88.1(5) . .
O2 W10 O14 156.6(5) . .
O4 W10 O14 85.8(5) . .
O30 W10 O21 169.9(4) . .
O3 W10 O21 72.4(5) . .
O2 W10 O21 85.3(5) . .
O4 W10 O21 84.2(4) . .
O14 W10 O21 72.2(5) . .
O30 W10 K4 84.7(4) . .
O3 W10 K4 136.3(3) . .
O2 W10 K4 130.2(3) . .
O4 W10 K4 45.2(3) . .
O14 W10 K4 48.6(4) . .
O21 W10 K4 95.0(3) . .
O9 W9 O19 102.9(6) . .
O9 W9 O2 103.6(6) . .
O19 W9 O2 90.9(5) . .
O9 W9 O1 99.9(6) . .
O19 W9 O1 157.1(5) . .
O2 W9 O1 84.6(5) . .
O9 W9 O26 99.3(5) . .
O19 W9 O26 88.8(5) . .
O2 W9 O26 156.6(5) . .
O1 W9 O26 86.6(5) . .
O9 W9 O31 170.2(6) . .
O19 W9 O31 72.1(5) . .
O2 W9 O31 85.1(4) . .
O1 W9 O31 85.2(4) . .
O26 W9 O31 72.5(4) . .
O9 W9 K3 56.8(5) . .
O19 W9 K3 50.6(4) . .
O2 W9 K3 119.0(4) . .
O1 W9 K3 148.7(3) . .
O26 W9 K3 78.1(4) . .
O31 W9 K3 115.2(3) . .
O9 W9 K2 83.7(4) . .
O19 W9 K2 132.7(4) . .
O2 W9 K2 133.7(4) . .
O1 W9 K2 49.3(3) . .
O26 W9 K2 44.2(4) . .
O31 W9 K2 93.5(3) . .
K3 W9 K2 103.41(10) . .
O44 W2 O6 101.6(5) . .
O44 W2 O42 100.4(6) . .
O6 W2 O42 89.7(5) . .
O44 W2 O1 101.5(5) . .
O6 W2 O1 89.0(5) . .
O42 W2 O1 157.9(5) . .
O44 W2 O4 100.0(5) . .
O6 W2 O4 158.3(5) . .
O42 W2 O4 87.9(5) . .
O1 W2 O4 85.3(5) . .
O44 W2 O25 171.7(5) . .
O6 W2 O25 73.1(4) . .
O42 W2 O25 73.6(5) . .
O1 W2 O25 85.0(4) . .
O4 W2 O25 85.6(4) . .
O44 W2 K4 82.0(4) . .
O6 W2 K4 136.4(4) . .
O42 W2 K4 47.4(4) . .
O1 W2 K4 133.5(3) . .
O4 W2 K4 48.9(3) . .
O25 W2 K4 97.4(3) . .
O44 W2 K2 87.6(4) . .
O6 W2 K2 46.5(4) . .
O42 W2 K2 136.1(4) . .
O1 W2 K2 48.4(3) . .
O4 W2 K2 133.5(3) . .
O25 W2 K2 93.0(3) . .
K4 W2 K2 169.56(11) . .
O22 W3 O36 100.1(5) . .
O22 W3 O15 102.0(5) . .
O36 W3 O15 86.9(5) . .
O22 W3 O8 97.4(5) . .
O36 W3 O8 91.6(5) . .
O15 W3 O8 160.5(5) . .
O22 W3 O26 100.0(5) . .
O36 W3 O26 159.7(5) . .
O15 W3 O26 86.6(5) . .
O8 W3 O26 88.2(5) . .
O22 W3 O31 167.9(5) . .
O36 W3 O31 86.5(4) . .
O15 W3 O31 88.4(5) . .
O8 W3 O31 72.1(5) . .
O26 W3 O31 74.2(4) . .
O22 W3 K1 79.4(4) . .
O36 W3 K1 50.7(4) . .
O15 W3 K1 136.4(3) . .
O8 W3 K1 49.6(4) . .
O26 W3 K1 136.7(4) . .
O31 W3 K1 97.5(3) . .
O22 W3 K2 84.8(4) . .
O36 W3 K2 132.4(4) . .
O15 W3 K2 46.3(3) . .
O8 W3 K2 135.1(3) . .
O26 W3 K2 47.7(3) . .
O31 W3 K2 98.3(3) . .
K1 W3 K2 164.12(9) . .
O39 W11 O28 102.4(6) . .
O39 W11 O33 99.5(5) . .
O28 W11 O33 95.5(5) . .
O39 W11 O36 101.2(5) . .
O28 W11 O36 91.2(5) . .
O33 W11 O36 156.3(5) . .
O39 W11 O38 93.9(5) . .
O28 W11 O38 162.9(5) . .
O33 W11 O38 86.7(5) . .
O36 W11 O38 80.5(5) . .
O39 W11 O34 172.0(5) . .
O28 W11 O34 81.8(5) . .
O33 W11 O34 73.1(4) . .
O36 W11 O34 85.4(4) . .
O38 W11 O34 82.6(4) . .
O39 W11 K1 90.0(4) . .
O28 W11 K1 48.6(3) . .
O33 W11 K1 144.1(3) . .
O36 W11 K1 47.4(3) . .
O38 W11 K1 127.4(3) . .
O34 W11 K1 97.9(3) . .
O45 Tb1 O7 81.7(4) . .
O45 Tb1 O37 72.4(4) . .
O7 Tb1 O37 129.2(4) . .
O45 Tb1 O28 124.4(4) . .
O7 Tb1 O28 80.4(4) . .
O37 Tb1 O28 79.7(4) . .
O45 Tb1 O11 143.0(4) . 3_676
O7 Tb1 O11 75.6(4) . 3_676
O37 Tb1 O11 144.1(4) . 3_676
O28 Tb1 O11 80.2(4) . 3_676
O45 Tb1 O46 73.2(4) . 3_676
O7 Tb1 O46 82.7(4) . 3_676
O37 Tb1 O46 127.2(4) . 3_676
O28 Tb1 O46 153.0(4) . 3_676
O11 Tb1 O46 75.3(4) 3_676 3_676
O45 Tb1 O46 93.1(4) . .
O7 Tb1 O46 147.5(3) . .
O37 Tb1 O46 78.1(4) . .
O28 Tb1 O46 126.9(4) . .
O11 Tb1 O46 90.8(4) 3_676 .
O46 Tb1 O46 65.2(4) 3_676 .
O45 Tb1 O32 135.4(4) . .
O7 Tb1 O32 142.9(4) . .
O37 Tb1 O32 73.4(4) . .
O28 Tb1 O32 75.4(4) . .
O11 Tb1 O32 72.9(4) 3_676 .
O46 Tb1 O32 107.3(4) 3_676 .
O46 Tb1 O32 52.1(4) . .
O45 Tb1 C1 114.8(5) . .
O7 Tb1 C1 157.6(4) . .
O37 Tb1 C1 72.3(5) . .
O28 Tb1 C1 100.2(5) . .
O11 Tb1 C1 82.4(5) 3_676 .
O46 Tb1 C1 87.7(4) 3_676 .
O46 Tb1 C1 26.9(4) . .
O32 Tb1 C1 25.4(4) . .
O45 Tb1 K1 118.6(3) . .
O7 Tb1 K1 127.7(3) . .
O37 Tb1 K1 46.7(3) . .
O28 Tb1 K1 47.8(3) . .
O11 Tb1 K1 98.4(3) 3_676 .
O46 Tb1 K1 147.1(3) 3_676 .
O46 Tb1 K1 82.9(2) . .
O32 Tb1 K1 41.6(3) . .
C1 Tb1 K1 59.4(3) . .
W5 O10 K1 152.3(6) . 2_645
W9 O9 Na1 165.6(8) . .
W9 O9 K3 95.7(6) . .
Na1 O9 K3 95.3(5) . .
W3 O8 W5 121.3(6) . .
W3 O8 K1 100.4(4) . .
W5 O8 K1 103.2(4) . .
W1 O7 Tb1 127.6(5) . .
W2 O6 W7 120.1(6) . .
W2 O6 Na2 129.2(6) . 3_575
W7 O6 Na2 97.2(5) . 3_575
W2 O6 K2 105.8(5) . .
W7 O6 K2 100.2(5) . .
Na2 O6 K2 99.3(4) 3_575 .
W10 O4 W2 151.6(7) . .
W10 O4 K4 106.7(4) . .
W2 O4 K4 100.8(4) . .
W10 O3 W8 122.8(6) . .
W10 O2 W9 153.9(7) . .
W9 O1 W2 153.1(6) . .
W9 O1 K2 102.1(4) . .
W2 O1 K2 103.2(4) . .
O32 K1 O83 74.0(4) . .
O32 K1 O39 98.4(4) . 2_645
O83 K1 O39 71.9(4) . 2_645
O32 K1 O10 117.1(4) . 2_655
O83 K1 O10 78.1(4) . 2_655
O39 K1 O10 124.2(4) 2_645 2_655
O32 K1 O8 111.8(4) . .
O83 K1 O8 144.8(4) . .
O39 K1 O8 72.8(4) 2_645 .
O10 K1 O8 123.0(3) 2_655 .
O32 K1 O36 108.9(4) . .
O83 K1 O36 158.9(4) . .
O39 K1 O36 126.7(4) 2_645 .
O10 K1 O36 82.2(3) 2_655 .
O8 K1 O36 54.8(3) . .
O32 K1 O37 60.1(3) . .
O83 K1 O37 128.5(4) . .
O39 K1 O37 91.8(3) 2_645 .
O10 K1 O37 142.5(4) 2_655 .
O8 K1 O37 53.1(3) . .
O36 K1 O37 66.1(3) . .
O32 K1 O28 61.2(3) . .
O83 K1 O28 117.3(4) . .
O39 K1 O28 150.3(3) 2_645 .
O10 K1 O28 85.4(3) 2_655 .
O8 K1 O28 94.0(3) . .
O36 K1 O28 52.8(3) . .
O37 K1 O28 59.8(3) . .
O32 K1 O49 162.7(4) . 2_655
O83 K1 O49 89.9(4) . 2_655
O39 K1 O49 82.3(3) 2_645 2_655
O10 K1 O49 51.5(3) 2_655 2_655
O8 K1 O49 85.0(4) . 2_655
O36 K1 O49 83.8(4) . 2_655
O37 K1 O49 137.2(4) . 2_655
O28 K1 O49 123.9(3) . 2_655
O32 K1 W3 124.5(3) . .
O83 K1 W3 160.7(3) . .
O39 K1 W3 98.0(3) 2_645 .
O10 K1 W3 95.4(3) 2_655 .
O8 K1 W3 29.9(2) . .
O36 K1 W3 29.2(2) . .
O37 K1 W3 66.8(2) . .
O28 K1 W3 79.7(2) . .
O49 K1 W3 72.2(3) 2_655 .
O32 K1 W5 82.3(3) . .
O83 K1 W5 134.9(3) . .
O39 K1 W5 74.3(3) 2_645 .
O10 K1 W5 146.9(3) 2_655 .
O8 K1 W5 29.6(2) . .
O36 K1 W5 65.5(2) . .
O37 K1 W5 26.0(2) . .
O28 K1 W5 81.2(2) . .
O49 K1 W5 114.3(3) 2_655 .
W3 K1 W5 52.48(6) . .
O32 K1 W11 86.5(3) . .
O83 K1 W11 134.6(3) . .
O39 K1 W11 152.8(3) 2_645 .
O10 K1 W11 75.1(3) 2_655 .
O8 K1 W11 80.5(3) . .
O36 K1 W11 29.6(2) . .
O37 K1 W11 67.4(2) . .
O28 K1 W11 25.6(2) . .
O49 K1 W11 100.9(3) 2_655 .
W3 K1 W11 58.50(7) . .
W5 K1 W11 79.93(9) . .
O82 K2 O15 145.4(5) . .
O82 K2 O26 122.3(5) . .
O15 K2 O26 55.4(3) . .
O82 K2 O27 121.8(5) . 4_585
O15 K2 O27 90.5(4) . 4_585
O26 K2 O27 67.3(3) . 4_585
O82 K2 O20 84.2(4) . 4_585
O15 K2 O20 96.7(4) . 4_585
O26 K2 O20 151.2(4) . 4_585
O27 K2 O20 110.4(4) 4_585 4_585
O82 K2 O6 92.8(4) . .
O15 K2 O6 55.0(4) . .
O26 K2 O6 92.3(3) . .
O27 K2 O6 145.2(4) 4_585 .
O20 K2 O6 73.8(3) 4_585 .
O82 K2 O1 86.9(4) . .
O15 K2 O1 64.3(3) . .
O26 K2 O1 53.2(3) . .
O27 K2 O1 119.8(3) 4_585 .
O20 K2 O1 125.4(3) 4_585 .
O6 K2 O1 53.0(3) . .
O82 K2 O29 112.7(4) . 4_585
O15 K2 O29 95.3(4) . 4_585
O26 K2 O29 115.0(4) . 4_585
O27 K2 O29 55.3(3) 4_585 4_585
O20 K2 O29 55.1(3) 4_585 4_585
O6 K2 O29 117.6(3) . 4_585
O1 K2 O29 159.6(4) . 4_585
O82 K2 W4 92.4(4) . 4_585
O15 K2 W4 103.6(3) . 4_585
O26 K2 W4 143.1(3) . 4_585
O27 K2 W4 84.8(2) 4_585 4_585
O20 K2 W4 26.3(2) 4_585 4_585
O6 K2 W4 98.3(3) . 4_585
O1 K2 W4 151.1(3) . 4_585
O29 K2 W4 30.3(2) 4_585 4_585
O82 K2 W3 149.7(4) . .
O15 K2 W3 29.4(2) . .
O26 K2 W3 30.0(2) . .
O27 K2 W3 67.8(2) 4_585 .
O20 K2 W3 121.3(3) 4_585 .
O6 K2 W3 80.4(3) . .
O1 K2 W3 65.4(2) . .
O29 K2 W3 96.3(3) 4_585 .
W4 K2 W3 117.71(14) 4_585 .
O82 K2 W1 118.1(4) . 4_585
O15 K2 W1 96.4(3) . 4_585
O26 K2 W1 90.6(3) . 4_585
O27 K2 W1 25.3(2) 4_585 4_585
O20 K2 W1 85.3(3) 4_585 4_585
O6 K2 W1 140.8(3) . 4_585
O1 K2 W1 143.8(3) . 4_585
O29 K2 W1 30.4(2) 4_585 4_585
W4 K2 W1 59.56(7) 4_585 4_585
W3 K2 W1 82.85(11) . 4_585
O82 K2 W7 122.7(4) . .
O15 K2 W7 28.7(3) . .
O26 K2 W7 80.4(2) . .
O27 K2 W7 115.5(3) 4_585 .
O20 K2 W7 75.1(2) 4_585 .
O6 K2 W7 30.3(3) . .
O1 K2 W7 65.4(2) . .
O29 K2 W7 97.7(2) 4_585 .
W4 K2 W7 91.25(11) 4_585 .
W3 K2 W7 57.86(8) . .
W1 K2 W7 112.67(14) 4_585 .
O84 K3 O86 168.2(4) . .
O84 K3 O85 72.5(4) . .
O86 K3 O85 95.7(4) . .
O84 K3 O24 93.4(4) . 4_575
O86 K3 O24 80.7(4) . 4_575
O85 K3 O24 61.4(4) . 4_575
O84 K3 O83 112.3(4) . 2_645
O86 K3 O83 79.2(4) . 2_645
O85 K3 O83 165.9(5) . 2_645
O24 K3 O83 129.5(4) 4_575 2_645
O84 K3 O19 76.7(4) . .
O86 K3 O19 105.4(4) . .
O85 K3 O19 97.7(4) . .
O24 K3 O19 158.9(4) 4_575 .
O83 K3 O19 71.5(4) 2_645 .
O84 K3 O32 81.2(4) . 2_645
O86 K3 O32 106.6(4) . 2_645
O85 K3 O32 125.2(4) . 2_645
O24 K3 O32 73.5(3) 4_575 2_645
O83 K3 O32 68.9(4) 2_645 2_645
O19 K3 O32 122.1(4) . 2_645
O84 K3 O9 109.0(4) . .
O86 K3 O9 64.8(4) . .
O85 K3 O9 67.1(4) . .
O24 K3 O9 113.2(4) 4_575 .
O83 K3 O9 98.9(4) 2_645 .
O19 K3 O9 55.1(3) . .
O32 K3 O9 166.7(4) 2_645 .
O84 K3 W9 87.7(3) . .
O86 K3 W9 89.0(3) . .
O85 K3 W9 75.0(3) . .
O24 K3 W9 133.7(3) 4_575 .
O83 K3 W9 91.6(3) 2_645 .
O19 K3 W9 29.4(2) . .
O32 K3 W9 151.5(3) 2_645 .
O9 K3 W9 27.5(2) . .
O84 K3 Na1 137.1(4) . .
O86 K3 Na1 33.1(3) . .
O85 K3 Na1 70.2(3) . .
O24 K3 Na1 87.0(3) 4_575 .
O83 K3 Na1 99.8(4) 2_645 .
O19 K3 Na1 87.9(3) . .
O32 K3 Na1 138.7(3) 2_645 .
O9 K3 Na1 35.6(3) . .
W9 K3 Na1 62.84(14) . .
O84 K3 K1 74.1(3) . 2_645
O86 K3 K1 117.7(3) . 2_645
O85 K3 K1 146.2(3) . 2_645
O24 K3 K1 115.9(3) 4_575 2_645
O83 K3 K1 42.7(3) 2_645 2_645
O19 K3 K1 79.6(3) . 2_645
O32 K3 K1 42.8(2) 2_645 2_645
O9 K3 K1 130.5(3) . 2_645
W9 K3 K1 108.86(12) . 2_645
Na1 K3 K1 142.52(18) . 2_645
O89 K4 O16 74.9(4) . 2_545
O89 K4 O30 73.4(4) . 2
O16 K4 O30 144.8(4) 2_545 2
O89 K4 O42 151.0(4) . .
O16 K4 O42 134.1(4) 2_545 .
O30 K4 O42 78.4(4) 2 .
O89 K4 O94 103.2(5) . 3_575
O16 K4 O94 93.6(4) 2_545 3_575
O30 K4 O94 79.4(4) 2 3_575
O42 K4 O94 77.8(4) . 3_575
O89 K4 O4 147.9(4) . .
O16 K4 O4 83.6(4) 2_545 .
O30 K4 O4 131.6(4) 2 .
O42 K4 O4 55.3(3) . .
O94 K4 O4 101.6(4) 3_575 .
O89 K4 O43 111.8(4) . .
O16 K4 O43 128.2(4) 2_545 .
O30 K4 O43 78.4(3) 2 .
O42 K4 O43 54.6(3) . .
O94 K4 O43 130.4(4) 3_575 .
O4 K4 O43 64.3(3) . .
O89 K4 O14 98.0(4) . .
O16 K4 O14 75.5(4) 2_545 .
O30 K4 O14 123.7(4) 2 .
O42 K4 O14 91.8(4) . .
O94 K4 O14 152.7(4) 3_575 .
O4 K4 O14 53.0(3) . .
O43 K4 O14 52.8(3) . .
O89 K4 W2 177.9(3) . .
O16 K4 W2 104.7(3) 2_545 .
O30 K4 W2 107.5(3) 2 .
O42 K4 W2 29.5(2) . .
O94 K4 W2 78.9(3) 3_575 .
O4 K4 W2 30.3(2) . .
O43 K4 W2 66.7(2) . .
O14 K4 W2 79.9(2) . .
O89 K4 W10 119.9(3) . .
O16 K4 W10 67.5(3) 2_545 .
O30 K4 W10 143.9(3) 2 .
O42 K4 W10 80.1(3) . .
O94 K4 W10 123.7(3) 3_575 .
O4 K4 W10 28.1(2) . .
O43 K4 W10 65.5(2) . .
O14 K4 W10 29.0(2) . .
W2 K4 W10 58.21(6) . .
O89 K4 W6 127.1(3) . .
O16 K4 W6 148.1(3) 2_545 .
O30 K4 W6 66.3(3) 2 .
O42 K4 W6 29.3(2) . .
O94 K4 W6 101.6(3) 3_575 .
O4 K4 W6 66.1(2) . .
O43 K4 W6 28.9(2) . .
O14 K4 W6 78.4(3) . .
W2 K4 W6 52.40(6) . .
W10 K4 W6 80.86(9) . .
O89 K4 W4 98.0(3) . .
O16 K4 W4 102.7(3) 2_545 .
O30 K4 W4 96.4(3) 2 .
O42 K4 W4 78.2(3) . .
O94 K4 W4 156.0(3) 3_575 .
O4 K4 W4 63.6(2) . .
O43 K4 W4 27.4(2) . .
O14 K4 W4 28.2(2) . .
W2 K4 W4 80.06(9) . .
W10 K4 W4 50.69(6) . .
W6 K4 W4 55.95(6) . .
O86 Na1 O9 83.9(5) . .
O86 Na1 O88 100.3(6) . .
O9 Na1 O88 90.8(6) . .
O86 Na1 O94 92.2(6) . .
O9 Na1 O94 94.3(6) . .
O88 Na1 O94 167.0(8) . .
O86 Na1 O44 177.9(5) . 3_575
O9 Na1 O44 97.2(5) . 3_575
O88 Na1 O44 81.5(6) . 3_575
O94 Na1 O44 86.0(5) . 3_575
O86 Na1 O93 84.2(5) . .
O9 Na1 O93 167.9(6) . .
O88 Na1 O93 89.1(6) . .
O94 Na1 O93 88.4(5) . .
O44 Na1 O93 94.7(5) 3_575 .
O86 Na1 Na2 94.3(4) . .
O9 Na1 Na2 132.5(4) . .
O88 Na1 Na2 42.7(5) . .
O94 Na1 Na2 133.2(5) . .
O44 Na1 Na2 86.2(4) 3_575 .
O93 Na1 Na2 46.5(4) . .
O86 Na1 Na2 61.1(4) . 3_565
O9 Na1 Na2 126.1(4) . 3_565
O88 Na1 Na2 60.4(5) . 3_565
O94 Na1 Na2 124.3(4) . 3_565
O44 Na1 Na2 119.3(5) 3_575 3_565
O93 Na1 Na2 44.6(3) . 3_565
Na2 Na1 Na2 33.6(3) . 3_565
O86 Na1 K3 40.2(3) . .
O9 Na1 K3 49.1(4) . .
O88 Na1 K3 114.9(6) . .
O94 Na1 K3 77.2(4) . .
O44 Na1 K3 139.9(4) 3_575 .
O93 Na1 K3 120.4(4) . .
Na2 Na1 K3 131.3(3) . .
Na2 Na1 K3 100.1(3) 3_565 .
O86 Na1 K4 119.5(4) . 3_575
O9 Na1 K4 113.4(4) . 3_575
O88 Na1 K4 134.4(6) . 3_575
O94 Na1 K4 33.0(4) . 3_575
O44 Na1 K4 58.4(3) 3_575 3_575
O93 Na1 K4 74.7(3) . 3_575
Na2 Na1 K4 108.6(2) . 3_575
Na2 Na1 K4 119.2(2) 3_565 3_575
K3 Na1 K4 110.0(2) . 3_575
Na2 Na2 O88 91.5(8) 3_565 .
Na2 Na2 O20 134.8(6) 3_565 2_545
O88 Na2 O20 75.4(6) . 2_545
Na2 Na2 O93 67.4(5) 3_565 .
O88 Na2 O93 79.9(6) . .
O20 Na2 O93 146.5(5) 2_545 .
Na2 Na2 O93 64.9(5) 3_565 3_565
O88 Na2 O93 101.1(6) . 3_565
O20 Na2 O93 75.3(4) 2_545 3_565
O93 Na2 O93 132.3(5) . 3_565
Na2 Na2 O6 143.5(7) 3_565 3_575
O88 Na2 O6 78.0(5) . 3_575
O20 Na2 O6 76.6(4) 2_545 3_575
O93 Na2 O6 76.3(4) . 3_575
O93 Na2 O6 151.1(5) 3_565 3_575
Na2 Na2 Na1 77.5(6) 3_565 .
O88 Na2 Na1 38.9(5) . .
O20 Na2 Na1 111.0(4) 2_545 .
O93 Na2 Na1 41.1(3) . .
O93 Na2 Na1 124.5(5) 3_565 .
O6 Na2 Na1 72.5(3) 3_575 .
Na2 Na2 Na1 68.9(5) 3_565 3_565
O88 Na2 Na1 139.3(5) . 3_565
O20 Na2 Na1 93.2(4) 2_545 3_565
O93 Na2 Na1 120.2(4) . 3_565
O93 Na2 Na1 38.6(3) 3_565 3_565
O6 Na2 Na1 138.0(5) 3_575 3_565
Na1 Na2 Na1 146.4(3) . 3_565
Na2 Na2 K2 156.2(7) 3_565 3_575
O88 Na2 K2 65.3(5) . 3_575
O20 Na2 K2 37.6(3) 2_545 3_575
O93 Na2 K2 110.8(4) . 3_575
O93 Na2 K2 112.7(4) 3_565 3_575
O6 Na2 K2 40.3(3) 3_575 3_575
Na1 Na2 K2 86.4(2) . 3_575
Na1 Na2 K2 125.3(3) 3_565 3_575
C1 O46 Tb1 136.0(11) . 3_676
C1 O46 Tb1 92.9(10) . .
Tb1 O46 Tb1 114.8(4) 3_676 .
W8 O45 Tb1 161.2(6) . .
W2 O44 Na1 125.7(6) . 3_575
W4 O43 W6 147.4(7) . .
W4 O43 K4 106.5(5) . .
W6 O43 K4 104.1(4) . .
W2 O42 W6 120.6(7) . .
W2 O42 K4 103.0(5) . .
W6 O42 K4 106.6(4) . .
W11 O39 K1 164.4(7) . 2_655
W7 O38 W11 153.8(7) . .
W5 O37 Tb1 155.7(7) . .
W5 O37 K1 105.5(5) . .
Tb1 O37 K1 98.6(4) . .
W3 O36 W11 155.0(7) . .
W3 O36 K1 100.2(4) . .
W11 O36 K1 103.1(4) . .
W8 O35 W4 120.5(5) . .
Ge1 O34 W1 124.2(6) . .
Ge1 O34 W11 124.1(5) . .
W1 O34 W11 95.6(4) . .
W11 O33 W1 117.1(6) . .
C1 O32 Tb1 92.9(11) . .
C1 O32 K1 124.1(10) . .
Tb1 O32 K1 101.6(4) . .
C1 O32 K3 124.0(12) . 2_655
Tb1 O32 K3 126.6(4) . 2_655
K1 O32 K3 88.6(3) . 2_655
Ge1 O31 W3 120.3(6) . .
Ge1 O31 W5 121.1(5) . .
W3 O31 W5 95.9(5) . .
Ge1 O31 W9 123.9(6) . .
W3 O31 W9 93.6(4) . .
W5 O31 W9 95.0(4) . .
W10 O30 K4 138.0(6) . 2_545
W4 O29 W1 156.5(6) . .
W4 O29 K2 93.5(4) . 4_586
W1 O29 K2 95.7(4) . 4_586
W11 O28 Tb1 129.8(6) . .
W11 O28 K1 105.8(4) . .
Tb1 O28 K1 97.2(4) . .
W1 O27 K2 108.7(5) . 4_586
W3 O26 W9 119.7(5) . .
W3 O26 K2 102.3(5) . .
W9 O26 K2 107.7(5) . .
Ge1 O25 W7 122.0(6) . .
Ge1 O25 W2 125.1(6) . .
W7 O25 W2 94.4(4) . .
Ge1 O25 W6 120.2(5) . .
W7 O25 W6 92.8(4) . .
W2 O25 W6 94.5(4) . .
W8 O24 K3 136.7(6) . 4_576
W5 O23 W8 143.6(7) . .
Ge1 O21 W4 120.7(6) . .
Ge1 O21 W8 119.5(6) . .
W4 O21 W8 94.7(4) . .
Ge1 O21 W10 125.4(5) . .
W4 O21 W10 93.8(4) . .
W8 O21 W10 95.4(4) . .
W4 O20 Na2 146.0(6) . 2
W4 O20 K2 105.0(5) . 4_586
Na2 O20 K2 107.7(4) 2 4_586
W9 O19 W5 123.0(6) . .
W9 O19 K3 100.0(4) . .
W5 O19 K3 129.0(6) . .
W6 O18 W7 118.7(6) . .
W6 O17 W1 154.0(6) . .
W6 O16 K4 148.8(6) . 2
W3 O15 W7 147.4(6) . .
W3 O15 K2 104.4(4) . .
W7 O15 K2 106.8(5) . .
W4 O14 W10 120.8(7) . .
W4 O14 K4 104.1(5) . .
W10 O14 K4 102.4(4) . .
O32 C1 O46 121.5(17) . .
O32 C1 C2 121.2(17) . .
O46 C1 C2 117.3(15) . .
O32 C1 Tb1 61.7(10) . .
O46 C1 Tb1 60.2(9) . .
C2 C1 Tb1 173.4(13) . .
Na1 O86 K3 106.7(5) . .
K1 O83 K3 93.4(5) . 2_655
Na1 O94 K4 119.9(7) . 3_575
Na1 O93 Na2 92.4(5) . .
Na1 O93 Na2 96.8(5) . 3_565
Na2 O93 Na2 47.7(5) . 3_565
Na1 O88 Na2 98.5(7) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W8 O24 1.746(11) .
W8 O45 1.767(12) .
W8 O23 1.939(11) .
W8 O35 1.939(12) .
W8 O3 2.051(12) .
W8 O21 2.299(11) .
W7 O41 1.686(11) .
W7 O38 1.810(12) .
W7 O15 1.936(12) .
W7 O18 1.962(12) .
W7 O6 1.979(12) .
W7 O25 2.281(11) .
W7 K2 3.858(5) .
W6 O16 1.734(13) .
W6 O17 1.790(12) .
W6 O18 1.920(12) .
W6 O43 1.958(10) .
W6 O42 2.009(12) .
W6 O25 2.331(11) .
W6 K4 3.931(4) .
W5 O10 1.752(12) .
W5 O37 1.767(11) .
W5 O23 1.913(12) .
W5 O8 1.971(11) .
W5 O19 2.047(12) .
W5 O31 2.299(12) .
W5 K1 3.885(4) .
W4 O20 1.714(12) .
W4 O43 1.889(10) .
W4 O29 1.892(12) .
W4 O14 1.923(12) .
W4 O35 1.946(11) .
W4 O21 2.289(11) .
W4 K2 3.739(4) 4_586
W4 K4 3.942(5) .
W1 O27 1.728(11) .
W1 O7 1.780(12) .
W1 O29 1.949(12) .
W1 O33 1.957(11) .
W1 O17 2.100(11) .
W1 O34 2.219(10) .
W1 K2 3.832(5) 4_586
Ge1 O34 1.716(11) .
Ge1 O25 1.741(11) .
Ge1 O21 1.759(11) .
Ge1 O31 1.767(11) .
W10 O30 1.708(12) .
W10 O3 1.832(11) .
W10 O2 1.900(12) .
W10 O4 1.923(10) .
W10 O14 1.945(12) .
W10 O21 2.315(12) .
W10 K4 3.912(5) .
W9 O9 1.712(13) .
W9 O19 1.840(12) .
W9 O2 1.920(11) .
W9 O1 1.922(11) .
W9 O26 1.939(12) .
W9 O31 2.336(11) .
W9 K3 3.691(5) .
W9 K2 3.920(4) .
W2 O44 1.710(12) .
W2 O6 1.905(12) .
W2 O42 1.910(12) .
W2 O1 1.926(11) .
W2 O4 1.936(10) .
W2 O25 2.306(11) .
W2 K4 3.775(4) .
W2 K2 3.951(4) .
W3 O22 1.712(12) .
W3 O36 1.870(11) .
W3 O15 1.918(12) .
W3 O8 1.917(12) .
W3 O26 1.940(12) .
W3 O31 2.265(11) .
W3 K1 3.778(4) .
W3 K2 3.788(5) .
W11 O39 1.701(12) .
W11 O28 1.763(11) .
W11 O33 1.928(11) .
W11 O36 1.989(10) .
W11 O38 2.077(12) .
W11 O34 2.256(11) .
W11 K1 3.929(4) .
Tb1 O45 2.302(13) .
Tb1 O7 2.327(11) .
Tb1 O37 2.364(11) .
Tb1 O28 2.374(11) .
Tb1 O11 2.408(12) 3_676
Tb1 O46 2.463(10) 3_676
Tb1 O46 2.470(11) .
Tb1 O32 2.506(13) .
Tb1 C1 2.843(19) .
Tb1 K1 4.103(4) .
O11 Tb1 2.408(12) 3_676
O10 K1 2.888(12) 2_645
O9 Na1 2.388(16) .
O9 K3 3.104(15) .
O8 K1 2.927(13) .
O6 Na2 2.980(15) 3_575
O6 K2 2.981(12) .
O4 K4 2.898(12) .
O1 K2 3.037(11) .
K1 O32 2.782(12) .
K1 O83 2.782(16) .
K1 O39 2.836(13) 2_645
K1 O10 2.888(12) 2_655
K1 O36 2.969(13) .
K1 O37 3.020(13) .
K1 O28 3.064(12) .
K1 O49 3.345(15) 2_655
K2 O82 2.602(18) .
K2 O15 2.825(12) .
K2 O26 2.867(12) .
K2 O27 2.911(14) 4_585
K2 O20 2.909(13) 4_585
K2 O29 3.112(12) 4_585
K2 W4 3.739(4) 4_585
K2 W1 3.832(5) 4_585
K3 O84 2.746(16) .
K3 O86 2.757(13) .
K3 O85 2.759(13) .
K3 O24 2.831(12) 4_575
K3 O83 2.843(14) 2_645
K3 O19 2.897(12) .
K3 O32 3.072(13) 2_645
K3 Na1 4.087(11) .
K3 K1 4.093(6) 2_645
K4 O89 2.752(15) .
K4 O16 2.782(13) 2_545
K4 O30 2.803(12) 2
K4 O42 2.854(13) .
K4 O94 2.890(15) 3_575
K4 O43 2.964(13) .
K4 O14 3.003(13) .
Na1 O86 2.328(15) .
Na1 O88 2.41(2) .
Na1 O94 2.420(16) .
Na1 O44 2.495(15) 3_575
Na1 O93 2.496(15) .
Na1 Na2 3.796(14) .
Na1 Na2 3.973(13) 3_565
Na1 K4 4.603(9) 3_575
Na2 Na2 2.25(2) 3_565
Na2 O88 2.60(2) .
Na2 O20 2.715(16) 2_545
Na2 O93 2.756(17) .
Na2 O93 2.809(15) 3_565
Na2 O6 2.980(15) 3_575
Na2 Na1 3.973(13) 3_565
Na2 K2 4.544(12) 3_575
O46 C1 1.29(2) .
O46 Tb1 2.463(10) 3_676
O44 Na1 2.495(15) 3_575
O39 K1 2.836(13) 2_655
O32 C1 1.219(19) .
O32 K3 3.072(13) 2_655
O30 K4 2.803(12) 2_545
O29 K2 3.112(12) 4_586
O27 K2 2.911(14) 4_586
O24 K3 2.831(12) 4_576
O20 Na2 2.715(16) 2
O20 K2 2.909(13) 4_586
O16 K4 2.782(13) 2
C1 C2 1.53(3) .
O83 K3 2.843(14) 2_655
O94 K4 2.890(15) 3_575
O93 Na2 2.809(15) 3_565
O49 K1 3.345(15) 2_645
